#------------------------------------------------------------------------------
#$Date: 2016-03-21 05:30:10 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178481 $
#$URL: svn://www.crystallography.net/cod/cif/4/03/02/4030275.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4030275
loop_
_publ_author_name
'Garcia-Martin, S.'
'Veiga, M. L. '
'Jerez, A.'
'Pico, C.'
'Santamaria, J.'
'Gonzalez-Diaz, G.'
_publ_section_title
;
 Synthesis and ionic conductivity of Rb(MoSb)O6
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              363
_journal_page_last               371
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'Mo O6 Rb Sb'
_chemical_formula_weight         399.16
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   10.2556(1)
_cell_length_b                   10.2556(1)
_cell_length_c                   10.2556(1)
_cell_volume                     1078.657(18)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.542
_exptl_absorpt_coefficient_mu    68.511
_exptl_crystal_density_diffrn    4.916
_exptl_crystal_density_meas      4.91
_refine_ls_R_I_factor            0.029
_cod_data_source_file            EJSSIC-1991-28-363-371.cif
_cod_data_source_block           Rb(MoSb)O6
_cod_original_cell_volume        1078.66(3)
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_database_code               4030275
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 x,y,z
2 -y,1/4+x,1/4+z
3 3/4-x,1/4-y,1/2+z
4 3/4+y,-x,3/4+z
5 x,1/4-y,1/4-z
6 3/4+y,1/4+x,1/2-z
7 3/4-x,y,3/4-z
8 -y,-x,-z
9 z,x,y
10 -x,1/4+z,1/4+y
11 3/4-z,1/4-x,1/2+y
12 3/4+x,-z,3/4+y
13 z,1/4-x,1/4-y
14 3/4+x,1/4+z,1/2-y
15 3/4-z,x,3/4-y
16 -x,-z,-y
17 y,z,x
18 -z,-y,-x
19 1/2-z,3/4+y,1/4+x
20 3/4+z,3/4+y,-x
21 1/4+z,-y,1/4+x
22 y,1/4-z,1/4-x
23 1/4-y,3/4-z,1/2+x
24 1/4-y,z,1/4-x
25 -x,-y,-z
26 y,3/4-x,3/4-z
27 1/4+x,3/4+y,1/2-z
28 1/4-y,x,1/4-z
29 -x,3/4+y,3/4+z
30 1/4-y,3/4-x,1/2+z
31 1/4+x,-y,1/4+z
32 y,x,z
33 -z,-x,-y
34 x,3/4-z,3/4-y
35 1/4+z,3/4+x,1/2-y
36 1/4-x,z,1/4-y
37 -z,3/4+x,3/4+y
38 1/4-x,3/4-z,1/2+y
39 1/4+z,-x,1/4+y
40 x,z,y
41 -y,-z,-x
42 z,y,x
43 1/2+z,1/4-y,3/4-x
44 1/4-z,1/4-y,x
45 3/4-z,y,3/4-x
46 -y,3/4+z,3/4+x
47 3/4+y,1/4+z,1/2-x
48 3/4+y,-z,3/4+x
49 x,1/2+y,1/2+z
50 -y,3/4+x,3/4+z
51 3/4-x,3/4-y,z
52 3/4+y,1/2-x,1/4+z
53 x,3/4-y,3/4-z
54 3/4+y,3/4+x,-z
55 3/4-x,1/2+y,1/4-z
56 -y,1/2-x,1/2-z
57 z,1/2+x,1/2+y
58 -x,3/4+z,3/4+y
59 3/4-z,3/4-x,y
60 3/4+x,1/2-z,1/4+y
61 z,3/4-x,3/4-y
62 3/4+x,3/4+z,-y
63 3/4-z,1/2+x,1/4-y
64 -x,1/2-z,1/2-y
65 y,1/2+z,1/2+x
66 -z,1/2-y,1/2-x
67 1/2-z,1/4+y,3/4+x
68 3/4+z,1/4+y,1/2-x
69 1/4+z,1/2-y,3/4+x
70 y,3/4-z,3/4-x
71 1/4-y,1/4-z,x
72 1/4-y,1/2+z,3/4-x
73 -x,1/2-y,1/2-z
74 y,1/4-x,1/4-z
75 1/4+x,1/4+y,-z
76 1/4-y,1/2+x,3/4-z
77 -x,1/4+y,1/4+z
78 1/4-y,1/4-x,z
79 1/4+x,1/2-y,3/4+z
80 y,1/2+x,1/2+z
81 -z,1/2-x,1/2-y
82 x,1/4-z,1/4-y
83 1/4+z,1/4+x,-y
84 1/4-x,1/2+z,3/4-y
85 -z,1/4+x,1/4+y
86 1/4-x,1/4-z,y
87 1/4+z,1/2-x,3/4+y
88 x,1/2+z,1/2+y
89 -y,1/2-z,1/2-x
90 z,1/2+y,1/2+x
91 1/2+z,3/4-y,1/4-x
92 1/4-z,3/4-y,1/2+x
93 3/4-z,1/2+y,1/4-x
94 -y,1/4+z,1/4+x
95 3/4+y,3/4+z,-x
96 3/4+y,1/2-z,1/4+x
97 1/2+x,y,1/2+z
98 1/2-y,1/4+x,3/4+z
99 1/4-x,1/4-y,z
100 1/4+y,-x,1/4+z
101 1/2+x,1/4-y,3/4-z
102 1/4+y,1/4+x,-z
103 1/4-x,y,1/4-z
104 1/2-y,-x,1/2-z
105 1/2+z,x,1/2+y
106 1/2-x,1/4+z,3/4+y
107 1/4-z,1/4-x,y
108 1/4+x,-z,1/4+y
109 1/2+z,1/4-x,3/4-y
110 1/4+x,1/4+z,-y
111 1/4-z,x,1/4-y
112 1/2-x,-z,1/2-y
113 1/2+y,z,1/2+x
114 1/2-z,-y,1/2-x
115 -z,3/4+y,3/4+x
116 1/4+z,3/4+y,1/2-x
117 3/4+z,-y,3/4+x
118 1/2+y,1/4-z,3/4-x
119 3/4-y,3/4-z,x
120 3/4-y,z,3/4-x
121 1/2-x,-y,1/2-z
122 1/2+y,3/4-x,1/4-z
123 3/4+x,3/4+y,-z
124 3/4-y,x,3/4-z
125 1/2-x,3/4+y,1/4+z
126 3/4-y,3/4-x,z
127 3/4+x,-y,3/4+z
128 1/2+y,x,1/2+z
129 1/2-z,-x,1/2-y
130 1/2+x,3/4-z,1/4-y
131 3/4+z,3/4+x,-y
132 3/4-x,z,3/4-y
133 1/2-z,3/4+x,1/4+y
134 3/4-x,3/4-z,y
135 3/4+z,-x,3/4+y
136 1/2+x,z,1/2+y
137 1/2-y,-z,1/2-x
138 1/2+z,y,1/2+x
139 z,1/4-y,1/4-x
140 3/4-z,1/4-y,1/2+x
141 1/4-z,y,1/4-x
142 1/2-y,3/4+z,1/4+x
143 1/4+y,1/4+z,-x
144 1/4+y,-z,1/4+x
145 1/2+x,1/2+y,z
146 1/2-y,3/4+x,1/4+z
147 1/4-x,3/4-y,1/2+z
148 1/4+y,1/2-x,3/4+z
149 1/2+x,3/4-y,1/4-z
150 1/4+y,3/4+x,1/2-z
151 1/4-x,1/2+y,3/4-z
152 1/2-y,1/2-x,-z
153 1/2+z,1/2+x,y
154 1/2-x,3/4+z,1/4+y
155 1/4-z,3/4-x,1/2+y
156 1/4+x,1/2-z,3/4+y
157 1/2+z,3/4-x,1/4-y
158 1/4+x,3/4+z,1/2-y
159 1/4-z,1/2+x,3/4-y
160 1/2-x,1/2-z,-y
161 1/2+y,1/2+z,x
162 1/2-z,1/2-y,-x
163 -z,1/4+y,1/4+x
164 1/4+z,1/4+y,-x
165 3/4+z,1/2-y,1/4+x
166 1/2+y,3/4-z,1/4-x
167 3/4-y,1/4-z,1/2+x
168 3/4-y,1/2+z,1/4-x
169 1/2-x,1/2-y,-z
170 1/2+y,1/4-x,3/4-z
171 3/4+x,1/4+y,1/2-z
172 3/4-y,1/2+x,1/4-z
173 1/2-x,1/4+y,3/4+z
174 3/4-y,1/4-x,1/2+z
175 3/4+x,1/2-y,1/4+z
176 1/2+y,1/2+x,z
177 1/2-z,1/2-x,-y
178 1/2+x,1/4-z,3/4-y
179 3/4+z,1/4+x,1/2-y
180 3/4-x,1/2+z,1/4-y
181 1/2-z,1/4+x,3/4+y
182 3/4-x,1/4-z,1/2+y
183 3/4+z,1/2-x,1/4+y
184 1/2+x,1/2+z,y
185 1/2-y,1/2-z,-x
186 1/2+z,1/2+y,x
187 z,3/4-y,3/4-x
188 3/4-z,3/4-y,x
189 1/4-z,1/2+y,3/4-x
190 1/2-y,1/4+z,3/4+x
191 1/4+y,3/4+z,1/2-x
192 1/4+y,1/2-z,3/4+x
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_thermal_displace_type
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_U_iso_or_equiv
Sb Sb Uiso 0.50000 0.50000 0.50000 0.500 0.0038
Mo Mo Uiso 0.50000 0.50000 0.50000 0.500 0.0053
O O Uiso 0.42500 0.12500 0.12500 1.000 0.0101
Rb Rb Uiso 0.10400 0.10400 0.10400 0.250 0.0060
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mo Mo -0.0483 2.7339 ' International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 ' International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.4688 1.6079 ' International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.0562 5.8946 ' International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O Sb O 85.14 10_655 15_555 yes
O Sb O 180.00 10_655 34_555 yes
O Sb O 94.86 10_655 39_565 yes
O Sb O 94.86 15_555 34_555 yes
O Sb O 180.00 15_555 39_565 yes
O Sb O 85.14 34_555 39_565 yes
O Mo O 85.14 10_655 15_555 yes
O Mo O 180.00 10_655 34_555 yes
O Mo O 94.86 10_655 39_565 yes
O Mo O 94.86 15_555 34_555 yes
O Mo O 180.00 15_555 39_565 yes
O Mo O 85.14 34_555 39_565 yes
Sb O Sb 134.02 26_555 49_544 yes
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sb O 1.9694(1) 10_655 yes
Sb O 1.9694(1) 15_555 yes
Sb O 1.9694(1) 34_555 yes
Sb O 1.9694(1) 39_565 yes
Mo O 1.9694(1) 10_655 yes
Mo O 1.9694(1) 15_555 yes
Mo O 1.9694(1) 34_555 yes
Mo O 1.9694(1) 39_565 yes
